Non-colloidal concentrated suspensions are frequently encountered in industrial process unit operations like pumping, mixing and transportation. Concrete, ceramics, composites, paint, and food products are some examples for industrial applications. From the processing side, it is important to predict the rheolog-ical properties of suspension systems as a function of various physical and chemical properties of the sus-pended particles and the ﬂuid as well. A clear goal for a food designer is, e.g. to produce low calorie, high solid content confectionery products, such as chocolates or nut pastes, with the same perceived textural properties as the full fat product. To tackle this problem, im-proved particle packing performance with reduced li-quid phase volume is an economically high potential
alternative to fat substitution by other ﬂuids (Villagran et al. 1996).
In recent decades, progress in theoretical description and experimental measurements was made for concen-trated suspensions containing monodisperse and poly-disperse particles. Suspensions containing monopoly-disperse spherical particles at high concentrations were studied intensively by various authors (Mooney 1951; Krieger and Dougherty 1959; Frankel and Acrivos 1967; Frith et al.1987; Buscall 1991; Schmidt and Mu¨nstedt2002). A number of studies focussed on concentrated bidisperse and polydisperse suspensions of spheres, and progress was reported (Farris 1968; Sudduth 1993; Chang and Powell 1994; Probstein et al. 1994; Gonderet and Petit 1997; Qin and Zaman 2003). Some experimental work was done to investigate the eﬀect of particle properties on the rheology of concentrated polydisperse Irene Marti
Oliver Ho¨ﬂer Peter Fischer Erich J. Windhab
Rheology of concentrated suspensions
containing mixtures of spheres and fibres
Received: 8 December 2004 Accepted: 9 December 2004 Published online: 12 March 2005 Springer-Verlag 2005
Abstract Optimising ﬂow properties of concentrated suspensions is an important issue common for many industries. The rheology of con-centrated suspensions has therefore been studied intensively both experimentally and theoretically. Most studies have focused on monodisperse and polydisperse suspensions of either spheres or ﬁbres. In practice, most suspensions contain particles that are polydis-perse both in size and shape. A mixing rule for such systems is expected to be a powerful tool for engineers and product designers. Therefore in this work, suspensions of spheres, ﬁbres and mixtures thereof were characterised using
rotational shear rheometry and in-line image analyses. Thereby, total solids volume concentration and ﬁbre fraction was varied. Results from transient and steady-state shear rheometry are discussed with respect to concentration, ﬁbre fraction, and shear induced micro-structure. Experimentally obtained viscosity data were accurately ﬁtted using the model proposed by Farris (T Soc Rheol 12:281, 1968) for mixtures of monodisperse
non-interacting spheres of diﬀerent sizes.
Keywords Sphere/ﬁbre suspen-sions Æ Mixing rules Æ Shape poly-dispersity
Originally presented at the Annual Euro-pean Rheology Conference 2003, AERC 2003
I. Marti Æ O. Ho¨ﬂer Æ P. Fischer (&) E. J. Windhab
Laboratory of Food Process Engineering, ETH Zentrum, ETH Zu¨rich,
Institute of Food Science and Nutrition, 8092 Zu¨rich, Switzerland
E-mail: peter.ﬁscher@ilw.agrl.ethz.ch Tel.: +41-1-6325349
suspensions (Dabak and Yucel 1986; Tsai et al.1992). Time-dependent rheology of concentrated suspensions is covered in the literature by concise reviews of Mewis (1979) and Barnes (1989, 1997). Theories of ﬁbre sus-pension rheology were recently reviewed by Petrie (1999). The description of ﬁbre orientation in ﬂow is the main objective of experimental studies carried out with concentrated ﬁbre suspensions (Stover et al. 1999; Barbosa et al. 1994). Experimental work treating the eﬀect of ﬁbre orientation on the rheology can also be found (Ganani and Powell 1985; Petrich et al. 2000). However, most suspensions encountered in practice are polydisperse, not only in size but also in shape. For the time being, a systematic investigation devoted to the problem of shape polydispersity cannot be found in the literature.
It is well established that the viscosity of suspensions increases as the solids volume concentration, cv,
in-creases (Mewis and Macosco 1993). The qualitative characteristics of the viscosity versus shear rate curves resemble the ones of the continuous phase at low-vol-ume fractions of about 1%. Increase in concentration leads to the occurrence of shear thinning at intermediate shear rates. At further increase of concentration, an apparent yield stress in the low shear rate regime be-comes evident. And at very high concentrations, approaching the maximum packing fraction, shear thickening can occur at high shear rates.
As the solids volume concentration is increased, suspended particles begin to interact, and the viscosity increases more than linearly with volume concentration. Interaction eﬀects can be accounted for by a power series expansion of the Einstein equation (Einstein 1906):
g¼ gsð1þ kEcvÞ ð1Þ
where g is the viscosity of the suspension, gs is the
vis-cosity of the continuous phase, cvis the solids volume
concentration, and kE is the Einstein coeﬃcient, which
equals 2.5 for non-interacting particles of spherical shape. Since higher order coeﬃcients are diﬃcult to calculate, semiempirical models are usually used for the description of concentrated suspensions. The volume fraction dependence of the low and high shear rate limiting relative viscosities, gr, is well described by the
Krieger–Dougherty equation (Krieger1972), see Eq. 2
gr¼ g gs¼ 1þ cv cv;max kcv;max ð2Þ
where k is a shape factor, and equals kEin Eq. 1. The
maximum packing fraction, cv,max, depends on the
physical characteristics of the particles, the particle size distribution, and the suspension structure.
Possibly, the most important factor aﬀecting the maximum packing fraction of highly concentrated
sus-pensions is the particle size distribution. Because smaller particles can ﬁt into the voids of bigger ones, the max-imum packing fraction increases gradually from mon-odispersed particle systems to polydispersed particle systems.
Two diﬀerent approaches are used in the develop-ment of predictive methods treating the problem of size distribution. In the eﬀective volume fraction approach, the maximum packing fraction is typically expressed as a function of particle size ratio, fraction of coarse parti-cles, and particle orientation factors (Windhab 2000). Derived equations have generally the form of Eq. 2. The second class is based on the separation of contribution parameters. Thereby, the contribution from parameters, such as ﬁne particles and coarse particles, are considered individually. The suspension viscosity is expressed as a combination of these parameters.
Farris (1968) was one of the ﬁrst investigators to deﬁne the relative viscosity as the contributions from ﬁne and coarse particles separately. According to his model, see Eq. 3, a bimodal system can be represented as a coarse fraction suspended in a matrix of ﬁne particles with the two fractions behaving independently of each other. To calculate the relative suspension viscosity, he assembled viscosity data of monodispersed distributions.
gr¼ g gs¼ gf gs g gf ¼ gfrgcr¼ H cv;f H cv;c ð3Þ
where gfris the relative viscosity of ﬁnes and is deﬁned as
the ratio of the viscosity of the suspensions containing just the ﬁne particles, gf, to the viscosity of the
sus-pending ﬂuid, gs. The relative viscosity of the coarse
fraction, gcr, is the contribution from the coarse
parti-cles. It is deﬁned as the ratio of the viscosity of the suspension, g, to the viscosity of the ﬁne fraction, gf. H is
the functional of corresponding variables. The volume fraction of the ﬁne particles, before adding the coarse particles to the suspension, and the volume fraction of coarse particles are labelled cv,f and cv,c, respectively.
For non-colloidal suspensions with non-interacting spherical particles, and where the size ratio of the sus-pended particles is greater than 10, excellent agreement between experiment and Farris model can be found (Qin and Zaman 2003). The maximum packing fraction of concentrated suspensions is very sensitive to the prop-erties of suspended particles and is controlled by the type of particle packing. When particles have irregular shapes, particle packing eﬃciency is expected to diﬀer from the case of spheres, and thus suspension viscosity is aﬀected.
In principle anisotropic particles such as ﬁbres, could be packed more tightly than spheres, although they would start to interact at lower concentrations. In real-ity, higher viscosities are normally found with aniso-tropic particles. The concentration dependency is
approximately exponential at low to moderate concen-trations, but still can be modelled using equations sim-ilar to Eq. 2. For suspensions of ﬁbres, the empirical value of cv, max was found to decrease roughly linear
with increasing ﬁbre aspect ratio (Metzner 1985). Fur-thermore due to hydrodynamic forces, anisotropic par-ticles tend to align in the direction of ﬂow. The packing density of such particle systems becomes, therefore, also a function of shear history (Barnes 1989; Windhab 2000).
The intention of this study is to characterise the inﬂuence of the total volume concentration and the ﬁbre fractions in the disperse phase on the ﬂow behaviour of suspensions made up with mixtures of spheres and ﬁ-bres. Rotational shear rheometry was used to investigate the transient eﬀect of shear deformation at constant applied shear rate as well as the eﬀect of shear rate on the viscous behaviour of the suspensions. In addition to the rheological characterisation, in-line image analysis was used as a tool to study the evolution of ﬁbre angle distribution as a function of applied shear treatment. It will be shown that for the studied suspensions systems the orientation behaviour of the ﬁbres is not aﬀected by the ﬁbre fraction. Fibre angle distribution is rather a function of shear history than a function of applied shear rate. To conclude, an attempt is made to model the viscous behaviour of the treated suspension systems. It will be demonstrated that the high shear rate relative viscosities of suspensions made up with mixtures of spheres and ﬁbres can be accurately ﬁtted using the Farris model.
Silicon oils (polydimethylsiloxanes) AK2000 and AK5000 obtained from Wacker-Chemie GmbH with a density of q25C=0.97 g cm)3and a zero shear viscosity
of g25 C=1.94 Pa s and 5.01 Pa s, respectively were
chosen as the suspending ﬂuids. The used oils exhibit Newtonian ﬂow behaviour up to a shear rate of around 1,000 s)1. The suspending ﬂuid was chosen in such a manner that no sedimentation occurred on the time scale of the longest measurements.
Hollow glass spheres from Potters Europe (Sphericel CP00) with a density of 1.1 g cm)3and glass ﬁbres from Vetrotex International (1304) with a density of 2.6 g cm)3were used as ﬁller particles. The ﬁbre diam-eter was chosen to correspond with the diamdiam-eter of the spheres. Distributions of ﬁbre diameter and length were obtained using image analysis, whereas a minimum of 1,000 measurements was assembled to calculate the distribution parameters. Micrographs were taken using an inverse light microscope (Diaphot-TMD, Nikon AG)
equipped with a 10· and a 20· objective, for ﬁbre diameter measurements and ﬁbre length measurements, respectively. Images were grabbed with a CCD-camera (3Cck Color Video Camera KY-F55B, JVC) on a Macintosh computer using a Quick Capture frame grabber card from Data Translation. Image grabbing and ensuing image analysis were performed using the public domain software NIH Image. The laser diﬀrac-tion instrument Malvern Masersizer-X was used to measure particle size distributions of the hollow glass spheres. The sample material was dispersed into deion-ised water using an ultrasound dispersing device (T480/ H-2, Elma). The dispersions were further diluted to a laser beam obscuration of 15–20%. Average size distri-bution parameters of the physical dimensions of the glass ﬁller particles are represented in Table1. The average ﬁbre aspect ratio results in 7.64.
In order to reduce eﬀects of adsorbed water on the surface of the hydrophilic ﬁller particles, they were dried in a vacuum oven at 130 C for 24 h before mixing. Suspension batches of 200 ml were prepared by immersing dried particles in silicon oil. The suspensions were mixed thoroughly with a stirrer for 2 h and stored in sealed containers. The ﬁbre length distribution was not aﬀected by mixing process. Fibre length distribu-tions were determined from samples before and after the mixing process. Statistical analysis of variance resulted in no signiﬁcant diﬀerence on level of conﬁdence of 1% between the samples taken before and after the mixing process. Prior to measurement, the suspensions were stirred again for several minutes. Entrapped air was re-moved in vacuum before starting the rheological experiments.
Rheological measurements were carried out at a con-stant temperature of 25 C using a strain-controlled rheometer (Rheometric Scientiﬁc ARES, Orchestrator 6.5.1 software). A Couette geometry with a cup diameter of 34 mm, a bob diameter of 32 mm, and a bob length of
Table 1 Distribution parameters of the physical dimensions of glass ﬁller particles (for ﬁbres r=0, and for spheres r=3) Physical dimension Average
xr,10(lm) Average xr,50(lm) Average xr,90(lm) Fibre diameter 11.3 13.3 15.3 Fibre length 42.3 101.5 164.7 Sphere diameter 4.7 11.7 26.7
33.2 mm was used. It has to be noted that the inﬂuence of gap width on the rheological data was checked beforehand. Fibre/sphere suspensions were measured using Couette geometries with gap widths up to 5 mm. After correcting the apparent shear rate data based on a stepwise power law approximation as described in (Eischen and Windhab 2002), the viscosity functions collapsed well and no systematic shift of the curves could be detected.
For the determination of the time dependent ﬂow behaviour, a constant shear rate was set and the inde-pendent variables were recorded as a function of time. Measurements were carried out in triplicate. For each run, a fresh sample was used.
Shear-rate dependent ﬂow behaviour was determined by collecting the independent variables ﬁrst at increasing and subsequently at decreasing shear rates. At each shear rate, the sample was allowed to equilibrate for 15 s and measurements were averaged during the succeeding 15 s. Before starting the rheological measurement, the suspensions were presheared at a shear rate of 0.5 s)1 and a preshear time of 2,000 s. Measurements were carried out in duplicate.
Determination of ﬁbre orientation in ﬂow
The evolution of ﬁbre orientation distribution in mixed glass sphere and glass ﬁbre suspensions was monitored using the RheoScope1 from Thermo Haake GmbH. The complete instrument (controlled stress rheometer, microscope, and CCD camera) is controlled by Rheo-Win software (Thermo Haake GmbH). Measurements were carried out at a constant temperature of 25 C using a polished cone geometry with a diameter of 70 mm and a cone angle of 0.981. For image acquisi-tion, a lens with optic magniﬁcation of 10· was used.
For the determination of the transient evolution of ﬁbre orientation, a constant shear rate of 1 s)1was set and the independent rheometric variables where re-corded over time. Simultaneously with the rheological measurement, the image information was acquired for each data point. With respect to the evolution of rheo-logical behaviour as a function of time, three time zones as indicated in Fig. 1were determined, in which orien-tation angles of the ﬁbres to the stream lines were assembled from ﬁve independent measurements. Image analysis was then performed on a Macintosh computer using the public domain software NIH Image.
The eﬀect of shear history on the ﬁbre angle distri-bution was evaluated by subjecting samples to step changes of shear rate (0.2, 0.5, 1, 5, and 10 s)1). Tests were performed in triplicate ﬁrst at increasing and sub-sequently at decreasing shear rates with and without prior preshear treatment (0.5 s)1 for 600 s). For each step, a holding time of 90 s was allowed, resulting in 90
measurements and images per applied shear rate of which the second half was used for image analysis.
Results and discussion
Characterisation of the pure ﬁbre and sphere suspensions
Before discussing the rheological behaviour of the mixed sphere/ﬁbre suspensions, suspensions made up of indi-vidual shape classes shall be reviewed brieﬂy. Viscosity as a function of solids volume concentration as well as time-dependent rheology will be discussed.
The results obtained for the viscosity measurements of suspensions of spheres and suspensions of ﬁbres with the experimental conditions described in the previous section are presented in Fig.2. A monotonic increase of the viscosities as the solids volume concentration, cv, is
increased can be seen for both suspension systems, with a strong increase as cvapproaches values around 0.6 and
0.4 for the sphere suspensions and the ﬁbre suspensions, respectively. This is a classical behaviour (Metzner 1985).
A standard way to model the volume concentration dependence of the relative viscosity of non-colloidal suspensions is to use a semiempirical model such as Eq. 2. The best ﬁt of our experimental relative upper Newtonian viscosities leads to the values of cv, max=0.64
and k=3.2 for the suspensions of spheres, and cv, max=0.43 and k=4.2 for the suspensions of ﬁbres.
Obtained values are in line with data reported in the literature for similar systems (Gonderet and Petit1997; Metzner 1985). If suspensions of hard spheres are
γ [-] ηr [-] 0 100 200 300 400 500 0 10 20 30 40 50 60 70 z1 z2 z3 z1: 15 s - 25 s z2: 50 s - 80 s z3: 420 s - 600 s
Fig. 1 Representation of the three time zones used for the determination of the ﬁbre angle alignment evolution at constant shear rate
ordered by ﬂow the value of cv, maxcan be larger and the
value of k is usually smaller (Gonderet and Petit1997). However, we will assume that the determined values are characteristic for the systems under investigation.
Figures3 and 4show the transient evolution of rel-ative viscosity as a function of shear deformation for suspensions with a total solids volume concentration of cv=0.2 for pure ﬁbres (cv=0.2, cv, f=1.0) and pure
spheres (cv=0.2, cv, f=0.0), respectively. Experiments
were carried out with conditions described in the previ-ous section and each displayed curve represents a mea-surement with a fresh sample.
The transient relative viscosity of the ﬁbre suspen-sions as a function of shear deformation is characterised by a steep rise at start-up of shear ﬂow and a decrease of viscosity after reaching the maximum viscosity. For large deformations, the viscosity levels oﬀ to an equi-librium value. This behaviour is characteristic for non-dilute ﬁbre suspensions (Barbosa et al. 1994). The rheopectic viscosity increase at the start up of shear ﬂow can be attributed to a combination of following eﬀects. (1) The formation of slip layers leads to very low start-up viscosity readings. (2) Fibre rotation is hindered through neighbouring ﬁbres. The resulting stiﬀening of the ﬁbre network leads to a viscosity increase. (3) Elastic properties in the ﬁbre network caused by strong inter-actions leads to delayed response of the sheared mate-rial. In semi-dilute long ﬁbre systems, increase in viscosity at small strains was found to be proportional on nL3, where L is the ﬁbre length and n the number of ﬁbres (Barbosa et al.1994). Furthermore, the maximum viscosity was shown to depend only on total shear deformation and not on the contributions from shear rate and time, separately. This is also the case in our experiments within the shear rate range of 1–10 s)1. Maximum viscosity as well as equilibrium viscosity ap-pears at same shear deformation values independent of the applied shear rate. However, in the experiment where a shear rate of _c = 0:5 s1was applied, maximum
viscosity is shifted to lower deformations and equilib-rium viscosity is only reached at larger deformations of
0.0 0.2 0.4 0.6 0 10 20 30 40 50 60 cv [-] ηr [-] spheres fibres
Fig. 2 Relative viscosities, gr, of suspensions of spheres (ﬁlled
circle) and ﬁbres (asterisk) as a function of the total solids volume concentration, cv high shear rate limit relative viscosities from
measurements at decreasing shear rates for suspensions of glass spheres and glass ﬁbres. Lines represent best ﬁt values given by the Krieger–Dougherty equation (Eq. 2) with cv, max=0.64 and k=3.2
for spheres, and cv, max=0.43 and k=4.2 for ﬁbres
0 10 20 30 40 50 0 2 4 6 γ [-] ηr [-] 10 s-1 5 s-1 1 s-1 0.5 s-1
Fig. 3 Transient relative viscosities as a function of shear defor-mation for a glass ﬁbre suspension with a solids volume concentration cv=0.2. Experimental results were obtained at four
diﬀerent shear rates _c¼ 0:5; 1; 2; 5; and 10 s1
0 10 20 30 40 50 γ [-] ηr [-] 10 s-1 5 s-1 1 s-1 0.5 s-1 0 1 2 3
Fig. 4 Transient relative viscosities as a function of shear defor-mation for a glass sphere suspension with a solids volume concentration cv=0.2. Experimental results were obtained at four
the sample material. In the second time segment of the curve, the viscosity decreases as a consequence of the orientation of the ﬁbres on the shear plane. Equilibrium viscosity is reached when no further increase in average ﬁbre orientation is reached through the ﬂow.
The sphere suspensions show weak time dependent behaviour at a total solids volume concentration of cv=0.2. Once the shear ﬂow was switched on, the
vis-cosity jumped to the equilibrium visvis-cosity value. If solids volume concentration of the sphere suspensions is in-creased, some time dependency becomes apparent, as shown in Fig. 5. Thus, increasing concentration leads to increased interactions between the particles and some structure changes take place in ﬂow. The thixotropy, however, is less pronounced than in the case of ﬁbre suspensions.
Time-dependent ﬂow behaviour of suspensions with mixtures of spheres and ﬁbres
In this section, the time-dependent ﬂow behaviour of suspensions with mixtures of ﬁbres and spheres will be discussed with respect to ﬁbre fraction and total solids volume concentration. The evolution of relative viscos-ity versus shear deformation from measurements with a constant shear rate of _c = 0:5 s1 which was well be-yond the limit where wall slip was evident is shown in Fig.6. Measurements were carried out using suspen-sions with a total solids volume concentration of cv=0.2, 0.3, 0.4, and 0.5. Within the given total cv the
volume concentration of ﬁbres cv, f were varied from
0.0 £ cv, f£ 1.0. For example, a suspension with cv=0.2
and cv, f=0.0 contains only spheres while a suspension
with cv=0.2 and cv, f=1.0 is purely consists our of
ﬁ-bres. In the mixed case, e.g. for cv=0.2 and cv, f=0.5
half of the total solids volume concentration are ﬁbres (cv=0.1) and spheres (cv=0.1). Before the samples were
ﬁlled into the rheometer cup, they were thoroughly stirred to achieve as random as possible ﬁbre orientation before the measurements. With increasing solids volume concentration, the maximum ﬁbre fraction allowing for rheological measurements decreased from and cv, f=1.0
(cv=0.2) to 0.33 (cv=0.5) as also indicates in Fig. 6. The
use of higher ﬁbre fractions resulted in highly viscous pastes and shear ﬂow was dominated by wall slip.
In general, with increasing the total solids volume concentration and increasing ﬁbre fraction more distinct time dependency can be observed, meaning that maxi-mum viscosity values and deformation necessary to reach equilibrium viscosity increase. A rheopectic in-crease in viscosity in the low shear deformation regime can only be found for suspensions with a ﬁbre volume concentration above a value of about cv, f=0.16. After
reaching the maximum viscosity value, these suspensions behave thixotropic over a long deformation range, which is much more pronounced than for pure ﬁbre suspensions (see Fig.3).
The most outstanding observation is the eﬀect of ﬁbre fraction on the equilibrium viscosity level. While for the suspensions with a total solids volume concentration of cv=0.2 and 0.3 (Fig.6a, b) the equilibrium viscosity is a
monotonic increasing function of ﬁbre fraction, this relationship changes at higher volume concentrations where increasing ﬁbre fractions ﬁrst lead to decreasing viscosity, and after passing a minimum at a ﬁbre fraction of cv, f=0.167 to increasing equilibrium viscosities at
further increase of ﬁbre fraction.
To evaluate whether the presence of spheres hindered the orientation of the ﬁbres in the shear ﬂow, experi-ments with the Rheoscope1 were carried out for sus-pensions with a total solids volume concentration of cv=0.5 and ﬁbre fractions from cv, f=0.125 to 0.33 with
experimental conditions as described in Materials and methods section. Figure7 shows exemplary for the suspension with a ﬁbre fraction of cv, f=0.33 the
evo-lution of ﬁbre angle distribution from time zone 1 to zone 3 (see Fig.1). An angle of 0 refers to a fully ori-ented ﬁbre, whereas an angle of 90 refers to a ﬁbre perpendicular to the direction of the ﬂow.
For an ideally random ﬁbre orientation, each orien-tation angle is equally possible. If the suspension is sheared ﬁbres start to rotate and align parallel to the streamlines (Barbosa et al.1994). Thus, with increasing shear deformation the ﬁbre angle distribution is ex-pected to shift from a ﬂat curve without distinctive maximum to a curve with a maximum at small angles. This kind of behaviour could be observed in all per-formed measurements. No dependency of ﬁbre fraction could be detected for the obtained results. This means
0 10 20 30 40 50 0.0 0.5 1.0 1.5 cv = 0.5 cv = 0.4 cv = 0.3 γ [-] ηr [-]
Fig. 5 Transient relative viscosities as a function of shear defor-mation for glass sphere suspensions with solids volume concentra-tions cv=0.3, 0.4, and 0.5. Experimental results were obtained at a
that ﬁbre rotation and alignment is not aﬀected by spherical particles in the suspension.
Shear-rate dependent ﬂow behaviour of suspensions with mixtures of spheres and ﬁbres
In the previous section, we demonstrated that for con-centrated suspensions with a solids volume concentra-tion of cv£ 0.3 the equilibrium relative viscosity at a
shear rate of _c = 0:5 s1 is an increasing monotonic
function of ﬁbre fraction. For highly concentrated sus-pensions with mixtures of spheres and ﬁbres and a solids volume concentration of cv‡0.4 the minimum
equilib-rium relative viscosities were measured at a ﬁbre fraction of around cv, f=0.167. However, the viscosity of
con-centrated suspensions is usually a function of shear rate and the slope in the shear thinning domain depends on concentration and on particle characteristics, such as size distribution and shape. Since measurements with a constant applied shear rate provide no information on the dependence on shear rate, results may be fragmentary, especially if the viscosity curves under
cv,f = 0.00 cv,f = 0.25 cv,f = 0.33 cv,f = 0.50 cv,f = 0.67 cv,f = 0.75 γ [-] ηr [-] 0 10 20 30 40 50 0 1 2 3 4 5 cv,f = 1.0 cv,f = 0.8 cv,f = 0.6 cv,f = 0.4 cv,f = 0.2 cv,f = 0.0 cv,f = 0.00 cv,f = 0.125 cv,f = 0.167 cv,f = 0.25 cv,f = 0.33 cv,f = 0.50 cv,f = 0.00 cv,f = 0.125 cv,f = 0.167 cv,f = 0.25 cv,f = 0.33 cv = 0.2 cv = 0.3 cv = 0.4 cv = 0.5 a b c d 0 20 40 60 80 100 0 10 20 30 40 0 20 40 60 80 100 0 10 20 30 40 50 0 20 40 60 80 100 0 20 40 60 80 100 γ [-] ηr [-] γ [-] ηr [-] γ [-] ηr [-]
Fig. 6 Transient relative vis-cosities as a function of shear deformation for suspensions with mixture of spheres and ﬁbres and solids volume con-centrations cv=0.2–0.5.
Exper-imental results were obtained at a shear rate of _c¼ 0:5; s1
Fig. 7 Distribution of the orientation angles for a suspension with a solids volume concentration of cv=0.5 and a ﬁbre fraction of cv, f=0.33 (corresponding to solid line in Fig.6d). Transient
measure-ments were obtained from image analysis performed with the Rheoscope 1 in time zones 1–3 according to Fig.1
consideration intersect. The aim of this section is to provide detailed information about the shear rate dependent ﬂow properties of suspensions with mixtures of spheres and ﬁbres. Measurements with experimental conditions described in the Materials section have been performed with suspensions in a concentration range of 0.2 £ cv£ 0.5 and ﬁbre fractions as used for the
inves-tigation of the transient ﬂow behaviour. Figure8shows the relative viscosity as a function of shear rate for these suspensions. All data points represent measurements obtained at decreasing shear rates from presheared samples, meaning that ﬁbres in the samples were ori-ented in shear ﬂow prior to measurements.
With a solids volume concentration of cv=0.2, ﬁbre
fractions ranging from 0£ cv, f£ 1 were used. The
resulting viscosity curves are shown in Fig.8a. They are characterised by shear thinning at low shear rates and an upper Newtonian viscosity plateau at a shear rate of around _c¼ 10 s1: The suspension of spheres
(cv, f=0) exhibits least pronounced shear thinning and
lowest viscosity. Both characteristics get more pro-nounced as the ﬁbre fraction increases. Furthermore,
with increasing ﬁbre fraction, the shear rate to reach the upper Newtonian viscosity plateau is slightly shifted to higher shear rates. If we raise the solids volume concentration to cv=0.3, similar characteristics for the
shear-rate dependency of viscosity can be found (see Fig.8b). Viscosity increases with increasing ﬁbre frac-tion, particularly at higher shear rates. However, at a solids volume concentration of cv=0.3 the slope of the
viscosity curve in the shear thinning regime is steeper for suspensions of spheres than for suspensions of ﬁ-bres. As a consequence, the slopes of the viscosity versus shear rate curve decrease with increasing ﬁbre fraction. At very low shear rates, the curves intersect. Thus, at the low shear rate limit, the suspension of ﬁbres and the suspension of spheres have about the same viscosity; and for the mixed suspensions, the viscosity at the low shear rate limit decreases with increasing ﬁbre fraction.
Further raising the total solids volume concentration to cv=0.4 and 0.5 leads to the shear-rate dependencies
of the viscosity as depicted in Fig.8c, d. The intersec-tion of the curves shifts to higher shear rates. At a
γ [s-1] . 6·100 cv,f = 0.4 cv,f = 0.2 cv,f = 0.0 cv,f = 0.8 cv,f = 0.6 cv,f = 1.0 cv = 0.2 a cv,f = 0.0 cv,f = 0.25 cv,f = 0.5 cv,f = 0.75 cv,f = 1.0 b ηr [-] cv,f = 0.0 cv,f = 0.167 cv,f = 0.25 cv,f = 0.5 cv = 0.4 c cv,f = 0.0 cv,f = 0.125 cv,f = 0.167 cv,f = 0.25 cv,f = 0.33 cv = 0.5 d 10-1 100 101 100 10-2 10-1 100 101 100 101 102 c v = 0.3 10-2 10-1 100 101 101 102 103 cv,f = 0.33 10-2 10-1 100 101 101 102 103 γ [s-1] . ηr [-] γ [s-1] . ηr [-] γ. [s-1] ηr [-]
Fig. 8 Relative viscosities as a function of shear rate for sus-pensions with mixture of spheres and ﬁbres and solids volume concentrations of cv=0.2–0.5. Experimental
re-sults were obtained at decreas-ing shear rates from presheared samples
concentration of cv=0.4, the upper Newtonian viscosity
of the suspension of spheres is still the lowest compared to the mixed suspensions, whereas in the case of solids volume concentration of cv=0.5 the minimum upper
Newtonian viscosity is obtained for the suspension with a ﬁbre fraction cv, f=0.167.
Measurements performed with the Rheoscope1 con-ﬁrmed that the degree of ﬁbre orientation was not the governing factor inﬂuencing the shear thinning behav-iour of the investigated suspension systems. Figure9 shows the evolution of the average ﬁbre angle, /50, 0, as
a function of the applied shear rate for suspensions with total solids volume concentration of cv=0.5 and various
This representation was chosen because no inﬂuence of ﬁbre fraction on the average orientation angle could be determined. Error bars indicate the standard devi-ation of the measured values. Standard devidevi-ation de-creased with measurement time, indicating that at the start-up of the measurement, the average ﬁbre angle depends on the initial ﬁbre orientation in the sample, which in practice is not ideally random (/50, 0„ 45).
This eﬀect gets balanced by applying preshear treat-ment before measuretreat-ment. However, the chosen pre-shear treatment was not suﬃcient to fully orient the ﬁbres. The average ﬁbre angle is a decreasing function of shear rate for measurement performed at increasing shear rates for both, presheared samples (open squares) and samples without preshear treatment (ﬁlled squares). Steady values were reached for shear rates
_c>2 s1: At ensuing measurements performed at decreasing shear rates (ﬁlled circles), average ﬁbre angle and its standard deviation remained roughly constant. Thus, the results show that spheres present in the sys-tem did not aﬀect the degree of ﬁbre orientation. As known for pure ﬁbre suspensions (Barbosa et al. 1994) also in suspensions with mixtures of spheres and ﬁbres as shown here, ﬁbre orientation is predominantly a function of shear history.
Application of the Farris model to predict the high shear rate viscosity of suspensions with mixtures of ﬁbres and spheres
In the previous section, the time-dependent and shear-rate dependent viscosities of suspensions made up with mixtures of ﬁbres and spheres were characterised by rotational rheometry and image analysis. We showed that with increasing concentration, the dependency of ﬁbre fraction on the relative high shear rate limit vis-cosity changes from a monotonically increasing behav-iour to the occurrence of a minimum viscosity level at intermediate ﬁbre fractions. Furthermore, image analy-sis showed that the degree of ﬁbre orientation was not a function of ﬁbre fraction for the investigated suspension systems.
The ﬂow behaviour of suspensions with mixtures of ﬁbres and spheres shows similarities to the properties of suspensions made up of fractions of ﬁne and coarse particles of spherical shape where the coarse particles are suspended in a ﬂuid made up of the suspension of ﬁne spheres. The viscosity of such suspensions can be modelled using Eq. 3, and good agreement between measurement and model is usually found for suspen-sions where the size ratio of suspended particles is high (Farris 1968; Qin and Zaman 2003). In our case, the suspended particles belong to diﬀerent shape classes. Based on the results from rheometry and in-line image analysis we can state that in shear ﬂow, the ﬁbres rotate freely in a suspension made up of spheres. Both, sus-pensions of spheres and sussus-pensions of ﬁbres were characterised with respect to their viscosity concentra-tion relaconcentra-tionships in the high shear rate regime. To recall, the diameter of the ﬁbres corresponds with the diameter of the spheres, and the average ﬁbre aspect ratio is 7.64.
Based on separate contributions from the suspensions of each shape class, the relative high shear rate limit viscosities of the mixed suspension systems were calcu-lated using Eq. 3, adopting ﬁbres as coarse particles. In Fig.10 results calculated from Farris’ model and rheo-logical measurements are displayed as a function of ﬁbre fraction for diﬀerent solids volume concentrations. They show excellent qualitative and quantitative agreement between model and experiment.
10-1 100 101 0 5 10 15 20 25 30 35 40 45 γ [s-1] φ50,0 [º]
Fig. 9 Average ﬁbre angle, /50,0, as a function of shear rate for
suspension with a solids volume concentration of cv=0.5 and
various ﬁbre fractions. (ﬁlled square) Measurements at increasing shear rates without preshear treatment. (open square) Measure-ments at increasing shear rates with preshear treatment. (ﬁlled circle) Measurements at decreasing shear rates after up-ramp from presheared samples. Error bars indicate standard deviations of average values
In this paper, the ﬂow behaviour of concentrated sus-pensions made up with mixtures of spheres and ﬁbres was investigated using shear rheometry and in-line im-age analysis. Both time-dependent and shear-rate
dependent ﬂow behaviour have been studied. Thereby solids volume concentration and ﬁbre fraction of the suspensions were varied systematically. We found that, time dependency and shear rate dependency is a function of solids volume concentration and ﬁbre fraction. At relatively low solids volume concentrations, the relative viscosity is a monotonic increasing function of the ﬁbre fraction. Raising the solids volume concentration leads to a minimum viscosity measured for suspensions with intermediate ﬁbre fractions. This minimum manifests in the low shear rate regime and shifts to higher shear rates with further increase of the solids volume concentra-tions.
Further it was demonstrated that the investigated suspension systems can be treated as suspensions of ﬁ-bres dispersed in a ﬂuid made up of the suspension of spheres. Based on the individual contribution from the suspensions of each shape class, the relative viscosities at the high shear rate limit were accurately ﬁtted using the model proposed by Farris (1968) for mixtures of monodisperse spheres of diﬀerent sizes. Thus, the results show the extended applicability of the Farris model for mixtures of particles from diﬀerent shape classes.
Acknowledgements The authors gratefully acknowledge Thermo Haake GmbH, Karlsruhe/Germany for providing Rheoscope 1 to acquire data for in-line image analysis. Financial support by the Commission for Technology and Innovation CTI, Bern/Switzer-land is acknowledged.
Barbosa SE, Ercoli DR, Bibbo´ MA, Kenny JM (1994) Rheology of short-ﬁbre composites: a systematic approach. Compos Str 27:83–91
Barnes HA (1989) Shear-thickening (‘‘dilatancy’’) in suspensions of nonag-gregating solid particles dispersed in Newtonian liquids. J Rheol 33:329–366 Barnes HA (1997) Thixotropy—a review. J Non-Newtonian Fluid Mech 70:1–33 Buscall R (1991) Eﬀect of long-range
repulsive forces on the viscosity of concentrated lattices: comparison of experimental data with an eﬀective hard sphere model. J Chem Soc Faraday Trans 87:1365–1370
Chang C, Powell RL (1994) Eﬀect of par-ticle size distribution on the rheology of concentrated bimodal suspensions. J Rheol 38:85–98
Dabak T, Yucel O (1986) Shear viscosity behaviour of highly concentrated sus-pensions at low and high shear rates. Rheol Acta 25:527–533
Einstein A (1906) Eine neue Bestimmung der Moleku¨ldimensionen. Ann Phys 19:289–306
Eischen J-C, Windhab EJ (2002) Viscosity of cocoa and chocolate products. Appl Rheol 12:32–34
Farris RJ (1968) Prediction of the viscosity of multimodal suspensions from uni-modal viscosity data. Trans Soc Rheol 12:281–301
Frankel NA, Acrivos A (1967) On the vis-cosity of a concentrated suspension of solid spheres. Chem Eng Sci 22:847–853 Frith WJ, Mewis J, Strivens TA (1987)
Rheology of concentrated suspensions: experimental investigations. Powder Technol 51:27–34
Ganani E, Powell RL (1985) Suspensions of rodlike particles—literature review and data correlations. J Compos Mater 19:194–215
Gonderet P, Petit L (1997) Dynamic vis-cosity of macroscopic suspensions of bimodal sized solid spheres. J Rheol 41:1261–1274
Krieger IM (1972) Rheology of monodis-perse lattices. Adv Colloid Int Sci 3:111–136
Krieger IM, Dougherty TJ (1959) A mechanism for non-Newtonian ﬂow in suspensions of rigid spheres. Trans Soc Rheol 3:137–152
Metzner AB (1985) Rheology of suspen-sions in polymeric liquids. J Rheol 29:739–775
Mewis J (1979) Thixotropy—a general re-view. J Non-Newtonian Fluid Mech 6:1–20
Mewis J, Macosco CW (1993) Suspension rheology. In: Macosco CW (ed) Rheol-ogy: principles, measurements and applications. VCH Publishers, New York, pp 425–474
Mooney M (1951) The viscosity of a con-centrated suspension of spherical parti-cles. J Colloid Sci 6:162–170
Petrich MP, Koch DL, Cohen C (2000) An experimental determination of the stress-microstructure relationship in semi-concentrated ﬁber suspensions. J Non-Newtonian Fluid Mech 95:101–133
Petrie CJS (1999) The rheology of ﬁbre suspensions. J Non-Newtonian Fluid Mech 87:369–402 0.0 0.2 0.4 0.6 0.8 1.0 100 101 102 cv,f [-] ηr [-] cv = 0.1 cv = 0.2 cv = 0.3 cv = 0.4 cv = 0.5 cv = 0.6 exp. values
Fig. 10 Relative viscosities as a function of ﬁbre fraction for suspensions with mixtures of spheres and ﬁbres. Lines represent calculated values from Farris’ model. (ﬁlled circle) Experimental results obtained at the high shear rate limit from suspensions at decreasing shear rates
Probstein RF, Sengun MZ, Tseng T-C (1994) Bimodal model of concentrated suspension viscosity for distributed particle sizes. J Rheol 38:811–829 Qin K, Zaman AA (2003) Viscosity of
concentrated colloidal suspensions: comparison of bidisperse models. J Colloid Int Sci 266:461–467
Schmidt M, Mu¨nstedt H (2002) Rheologi-cal behaviour of concentrated mono-disperse suspensions as a function of preshear conditions and temperature: an experimental study. Rheol Acta 41:193–204
Stover CA, Koch DL, Cohen C (1992) Observation of ﬁbre orientation in simple shear ﬂow of semi-dilute sus-pensions. J Fluid Mech 238:277–296 Sudduth RD (1993) A new method to
pre-dict the maximum packing fraction and the viscosity of solutions with a size distribution of suspended particles. J Appl Polym Sci 48:37–55
Tsai SC, Botts D, Plouﬀ J (1992) Eﬀects of particle properties on the rheology of concentrated noncolloidal suspensions. J Rheol 36:1291–1304
Villagran FV, McCabe GM, Wong VYL (1996) Process for making reduced fat nut spreads US Patent 5,490,999. Procter & Gamble Co, Cincinnati, OH, USA
Windhab EJ (2000) Fluid immobiliza-tion—a structure-related key mecha-nism for the viscous behavior of concentrated suspension systems. Appl Rheol 10:134–139